4Kossel Technique:This technique is based on using electron beam to generate X-rays within the sample under investigation.Need high acceleration voltage. About 2-3 times larger than the critical voltage to produce characteristic X-ray K radiation.The X-rays are subjected to subsequent reflection at the lattice planes of the sample in accordance with Bragg’s law to form cone shapes - Kossel cones.These are recorded on an X-ray sensitive film (see Fig. next slide).
5(a) Diagram illustrating the formation of Kossel patterns in reflection; (b) Kossel pattern from titanium(a)(b)
6Because the wavelength of X-rays (Kossel technique) is much larger than that of electrons, all Bragg angles between 0o and 90o may occur.Therefore the resulting projection lines on the film plane are strongly curved as seen in Figure 22(b).
7Electron Channeling Pattern (ECP): Can be used to determine crystallographic orientation, structural type (image contrast), unit cell size, or a measure of the crystal perfection.Although we cannot obtain diffraction spot patterns in the SEM, as we can in the TEM, we can make use of electron channeling for diffraction patterns.
8For orientation determination, the electron beam in the SEM is focused on the sample site to be analyzed.The beam is tilted at this position by an angle , and rocked on the specimen surface, as shown in Figure, next slide.
10The resulting pattern is known as selected area channeling pattern (SACP). Although there method of formation are not identical, the SACPs are geometrically similar to TEM Kikuchi patterns and EBSD patterns.Therefore, they are analyzed in a similar manner.They are composed of bright bands of a given thickness representing distinct crystallographic planes (see Figs. next slides).
12Electron channel pattern obtained from a gallium phosphide crystal of (111) orientation.
13Electron channel pattern of a recrystallized grain in a partially recrystallized Al-Fe-Si sample.
14In general, the spatial resolution of this technique is limited to 10 m. Also, the technique is very sensitive to lattice defects. Therefore, only recrystallized or recovered microstructures have been successfully analyzed.
15It is also possible to obtain channeling contrast for structural information. Channeling contrast is generally much weaker than atomic number contrast. Therefore contrast is low.Good electron detector, a carefully prepared specimen and large beam currents are usually required in order to improve the contrast.
16Electron Backscattered Diffraction (EBSD): Can be considered as the most widely used microtexture technique.Generation of PatternsBackscattered electrons are produced when stationary beam (scan coils are turned off) are incident on a specimen (in the SEM) that is tilted to a about 70o (see next Figure).
17Schematic diagram showing the specimen-beam interaction volume in a specimen tilted for EBSD
18The Interaction Volume of Backscattered Electrons x 2 times the spot sizeSpot Size: 30nm15kV, 60m Aperturey 2.5 to 3 times the spot sizePenetration depth (z):50 – 100nmWhen Considering the Issue of Interaction Volume\Penetration Depth:Will the beam penetrate through the precipitates?Will there be pattern overlapping from Austenite Matrix?
19The main effect of tilting the specimen is to reduce the path length of electrons, which have been backscattered by lattice planes.Therefore, when compared to flat specimen, more of these electrons undergo diffraction, and escape from the specimen before being absorbed.
20The electrons that contribute to the pattern are only those: The EBSD pattern results from diffraction of a divergent source of electrons generated within the sample just beneath the point where the primary electron strikes the specimen.The electrons that contribute to the pattern are only those:That have lost no more than a few electron volts of energy.Emerge from a depth in the specimen of no more than 30 to 40 nanometers, which is a considerably smaller depth than that reached by the primary beam.
21The large beam current can be countered by using: The lower the primary beam voltage, the better the resolution, because the beam spread is smaller.This benefit may be offset, because at lower primary voltages, the probe diameter for a given current is lager.The large beam current can be countered by using:Field emission source, orLower beam currents. However, lower beam current leads to a poorer signal to noise ratio.
22Detection of PatternsThe diffraction pattern can be captured on a recording medium or device placed in front of the tilted specimen.Examples of detecting or recording medium are:a phosphor screen, viewed by a low light television camera. The luminosity of a phosphor screen for a beam current of 100 pA at 20 kV is of the order of 10-4 lux (10 times greater than that detectable in live TV by a SIT camera.CCD camera, which produces about 50 times more luminosity than a phosphor screen.Next Figure shows a schematic of the specimen and the detecting medium.
23Schematic of a tilted specimen and a detecting medium.
25Image processing involves integration of successive patterns and background subtraction, which are used to improve the signal to noise ratio.The above reduces the dynamic range to between gray level 90 and gray level Sharper and higher order lines are usually lost in this process.Further image processing is performed to reduce the number of pixels in the image to approximately 10,000. This enables the computer analysis of the pattern, namely the Hough transform, to be executed in a fraction of a second.
29EBSD Specimen Preparation: A carefully prepared specimen, with no deformed surface (top nm) layer.Specimen preparation is supposed to be uncomplicated, and similar to that for optical microscopy.Since the diffraction zone is shallow, the specimen surface must no be obscured by:mechanical damage due to grinding,surface layers due to thick coatings,surface undulation due to protruding particles, orcontamination
30Minimization of diamond polishing is necessary in order to avoid surface damage. It may be necessary to avoid some common electropolishes or etchants, which may deposit films on the surface. A useful guide is to use TEM electrolytes.A combination of etching and mechanical polishing may be used, especially if OIM is required.Final polish in colloidal silica is highly recommended.
31Inadequate or inappropriate specimen preparation could give rise to erroneous data interpretation. Acceleration voltage and coating of samples can affect the quality of diffraction pattern obtained, as can be seen in the next Figure (a) - (c).
32Effect of acceleration voltage on the quality of diffraction pattern of sample with no coating (a) 10 kV accelerating voltage and (b) 40 kV accelerating voltage.
33Effect of acceleration voltage on the quality of diffraction pattern of a coated (5 nm Ni) sample (c) 10 kV accelerating voltage and (d) 40 kV accelerating voltage.
34Some Specimen Preparation Methods Heavily Deformed OFHC Copper Mechanical polishLight diamond polishSilica on Vibromet polishEtch in 50% Ammonium Hydroxide and 50% Peroxide
35Commercially pure aluminum, titanium alloys Mechanical polishLight diamond polishElectropolish in 5% perchloric acid in ethanol at -25oCAluminum-lithium alloysImmerse for several seconds in Keller’s reagent, slightly warmed.
36Mild Steel Mechanical polish Light diamond polish Swab with 2% nital for several seconds
37Limitations of EBSD Technique: Materials with very fine grain/subgrain size.e.g. Nanocrystalline material - can be resolved by employing the TEM-based microtexture technique.Materials that have undergone extensive deformation.e.g. heavily cold worked material by wire drawing - may resolve through novel polishing technique.
38Resolution and Operation Parameters: The absolute spatial resolution of EBSD technique depends on the interaction volume of the electron beam and the specimen, which in turn depends on the spot size. Quoted values are:average spatial resolution is about 200 to 500 nmaccuracy is about 1oThe above parameters are influenced by:MaterialSpecimen/microscope geometryAccelerating voltageProbe currentPattern clarity
39Specimen/Microscope geometry MaterialBackscattered signal increases with atomic number. Therefore, better patterns are generally obtained from materials with high atomic number elements.Specimen/Microscope geometryspecimen tilt angle must be about 70oMaintain short working distance, and this will depend on the geometry of the microscope.Specimen to screen distance. This is fixed for each microscope - camera pair.
40Accelerating voltage Probe current There is a linear relationship between accelerating voltage and interaction volume for every element. One needs to find an optimum accelerating voltage, and this can always be compensated/complemented with probe current.Probe currentThis is usually selected in accordance with the light sensitivity of the camera.
41Orientation Imaging Microscopy (OIM): An Orientation Imaging Micrograph is produced by successively collecting and indexing Electron Backscattered Diffraction (EBSD) patterns at point spaced over a specimen surface in a regular grid.The technique is based on electron backscattered diffraction in the scanning Electron microscope.